Presentation on theme: "Dr. Waseem Bahjat Mushtaha Specialized in prosthodontics"— Presentation transcript:
1 Dr. Waseem Bahjat Mushtaha Specialized in prosthodontics Dental Casting AlloysDr. Waseem Bahjat MushtahaSpecialized in prosthodontics
2 Dental Casting AlloysCasting is the most commonly used method for the fabrication of metal structures (inlays, crowns, partial denture frames. A pattern of the structure is first made in wax. This is then surrounded by an investment material. After the investment hardens, the wax is removed (burnt out) leaving a space or mould. Molten alloy is forced into this mould. The resulting structure is an accurate duplication of the original wax pattern.
3 TERMINOLOGYAlloy : An alloy is defined as a metal containing two or more elements, at least one of which is metal, and all of which are mutually soluble in the molten state.
4 Classification of alloys According to Use :1) Alloys for all metal and resin veneer restorations" (e.g. inlays, posts, resin and composite veneered crowns & bridges) ) Alloys for metal ceramics restorations
5 According to Yield Strength and Percentage Elongation (ADA Sp According to Yield Strength and Percentage Elongation (ADA Sp. 5 Classification)Type I SoftType II MediumType III HardType IV Extra hard
6 According to Nobility (ADA 1984) A. High noble metal alloysContains greater or equal 40 wt% Au and greater or equal 60 wt% of noble metalsB. Noble metal alloysContains greater or equal 25 wt% of noble metalsC. Predominantly base metalContains less than 25 wt% of noble metals
7 According to Major Element 1- Gold alloys2-Silver alloys3-Palladium alloys4-Nickel alloys5-Cobalt alloys6-Titanium alloys
8 According to the Three Major Elements 1-Gold-palladium-silver2- Palladium-silver-tin3- Nickel-chromium-molybdenum4- Cobalt-chromium-molybdenum5-Iron-nickel-chromium6- Titanium-aluminum-vanadium
9 According to the Number of Alloys Present 1) Binary-two elements 2) Ternary-three elements3) Quaternary (and so forth)-four elements
10 General Requirements of Casting Alloys All cast metals in dentistry have some basic common requirements1)They must not tarnish and corrode in the mouth.2) They must be sufficiently strong for the intended purpose.3)They must be biocompatible (non-toxic and non-allergic).4)They must be easy to melt, cast, cut and grind (easy to fabricate).5)They must flow well and duplicate fine details during casting.6)They must have minimal shrinkage on cooling after casting. 7)They must be easy to solder.
11 Not all of them meet all the requirements Not all of them meet all the requirements. Some have shown a potential for allergic reactions (nickel containing alloys) and other side effects when used without proper precautions. Some are quite difficult to cast. Some are so hard (base metal alloys) that they are difficult to cut, grind and polish. All alloys shrink on cooling. Some (base metal alloys) show more shrinkage than others. The shrinkage cannot be eliminated but it can be compensated for (investments). Besides these general requirements, alloys intended for a certain specific use must meet requirements for that. For example metal ceramic alloys must have additional requirements in order to be compatible with porcelain.
12 ALLOYS FOR ALL METAL RESTORATIONS These alloys were among the earliest alloys available to dentistry. The early alloys were mostly gold alloys. Since they were intended for all metallic and later for resin veneered restorations, they just had to meet the basic requirements. No special requirements are needed for veneering with resin. Currently, the use of these alloys are slowly declining because of the:1) Increased esthetic awareness has reduced the trend for metal display. 2)Increasing popularity of all ceramic and metal ceramic restorations. 3)Reducing popularity of resin and composite as veneering material.Resing facings have a number of disadvantages.- They wear rapidly (soon wear resistance)- They may change color (color instability and stain absorption)- They are porous. They tend to absorb food material and bacteria. This makes it unhygienic and gives it a bad odor.
13 Classification(As mentioned before this 1934 classification was originally intended for gold alloys and were based on hardness. Since 1989, it was relaxed to include any dental alloy as long as they met the new yield strength and percentage elongation criteria).Type I SoftSmall inlays, class III and class V cavities which are not subjected to great stress. They are easily burnished. These being highly malleable and ductile have self-sealing margins like gold foil filling.Type II MediumInlays subject to moderate stress, thick 3/4 crowns, abutments, pontics, full crowns, and sometimes soft saddles. They are less resistance to tarnish and corrosion than type I they are not self-sealing like type I gold alloys.Type III HardInlays, crown and bridges, situations where there may be great stresses involved. They usually can be age hardened.Type IV Extra Hard Inlays subjected to very high stresses, partial denture frameworks and long span bridges. They can be age hardened. These are less resistant to tarnish and corrosion than type I,II and III alloys.
14 Types These alloys will be discussed under the following categories High noble (gold alloys)Noble (Silver palladium alloys)Base metalCobalt chrome alloys-Titanium and its alloys Aluminum bronze alloys
15 GOLD ALLOYS (FOR ALL METAL RESTORATIONS) Synonyms:Traditional gold alloys, Au-Ag-Cu alloys.
16 Why do We Alloy Gold?Pure gold is a soft and ductile metal and so is not used for casting dental restorations and appliances. Dental casting golds are alloyed commonly with copper, silver, platinum, nickel and zinc. Alloying gold with these metals not only improves its physical and mechanical properties but also reduces its cost. Earlier, people liked to display the yellow color of gold probably as a symbol of social status. Currently, the trend is to avoid display of metal. At the same time, increase in the platinum, palladium and silver content of modern alloys have resulted in whiter colored gold alloys. Thus, there are 'yellow gold alloys' and 'white gold alloys'. The rise in gold prices have also led to the availability of alloys with low gold content. These are the 'low golds
17 GOLD CONTENTTraditionally, gold content of dental casting alloys was called:1)Karat2)Fineness.KaratIt refers to the parts of pure gold present in 24 parts of alloy, e.g.- 24 karat gold is pure gold.- 22 karat gold is 22 parts pure gold and 2 parts of other metal." FinenessFineness of a gold alloy is the parts per thousand of pure gold. Pure gold is 1000 fine. Thus, if 3/4 of the gold alloy is pure gold, it is said to be 750 fine.
18 Function of Each Element (gold alloys) Provides tarnish and corrosion resistance and has a desirable appearance. Also provides ductility and malleability.Copper :It is the principal hardener. It reduces the melting point and density of gold. If present in sufficient quantity, it gives the alloy a reddish color. It also helps to age harden gold alloys. In greater amounts it reduces resistance to tarnish and corrosion of the gold alloy. Therefore, the maximum content should not exceed 16 percent.
19 Silver :It whitens the alloy, thus helping to counteract the reddish color of copper. It increases strength and hardness slightly. In large amount, however, it reduces tarnish resistancePlatinum :It increases strength and corrosion resistance. It also increases melting point and has a whitening effect on the alloy. It helps to reduce the grain size.
20 Palladium :Similar to platinum in its effect. It hardens and whitens the alloy. It also raises fusion temperature and provides tarnish resistance. It is less expensive than platinum, thus, reducing the cost of the alloy.
21 The Minor Additions Zinc : It acts as a scavenger for oxygen. Without zinc, the silver in the alloy causes absorption of oxygen during melting. Later during solidification, the oxygen is rejected producing gas porosities in the casting.
22 Indium, Tin and Iron :They help to harden the ceramic gold- palladium alloys, iron being the most effective.Calcium :It is added to compensate for the decreased CTE that results when the alloy is made silver free (The elimination of silver is done to reduce the tendency for green stain at the metal-porcelain margin).
23 Iridium, Ruthenium, Rhenium They help to decrease the grain size. They are added in small quantities.Note All modern noble metal alloys are fine grained. Smaller the grain size of the metal, the more ductile and stronger it is. It also produces a more homogeneous casting and improves the tarnish resistance. A large grain size reduces the strength and increases the brittleness of the metal. Factors controlling the grain size are the rate of cooling, shape of the mould, and composition of the alloy.
24 PROPERTIES OF GOLD ALLOYS Color :Traditionally the gold alloys were gold colored. The color of modern gold alloys can vary from gold to white. It depends on the amount of whitening elements (silver, platinum, palladium, etc.) present in the alloy.
25 Melting Range :Ranges between 920 to 960°C. The melting range of an alloy is important. It indicates the type of investment required and the type of heating source needed to melt the alloy.Density :It gives an indication of the number of dental castings that can be made from a unit weight of the metal. In other words, more number of cast restorations per unit weight can be made from an alloy having a lower density, than one having a higher density. Gold alloys are lighter than pure gold (19.3 gms/cm').Type III gm/cm:‘Type IV gm/cm'The castability of an alloy is also affected by density. Higher density alloys cast better than lower density alloys.
26 Yield strength:The yield strength for :Type III – 207 MPa.Type IV- 275 MPaHardness :The hardness forType III- 121 MPaType IV- 149 MPa.The hardness indicates the ease with which these alloys can be cut, ground or polished. Gold alloys are generally more user friendly than the base metal alloys which are extremely hard.
27 ElongationIt indicates the ductility of the alloy. A reasonable amount is required especially if the alloy is to be deformed during clinical use, e.g. clasp adjustment for removable partial dentures, margin adjustment and burnishing of crowns and inlays. Type I alloys are easily furnished. Alloys with low elongation are very brittle. Age hardening decreases ductility: Type III - 30 to 40%Type IV - 30 to 35%.
28 Modulus of Elasticity This indicates the stiffness/flexibility of the metal. Gold alloys are more flexible than base metal alloysTarnish and Corrosion Resistance Gold alloys are resistant to tarnish and corrosion. This is due to their high noble metal content. Noble metals are less reactive.
29 Casting ShrinkageAll alloys shrink when they change from liquid to solid. The casting shrinkage in gold alloys is less (1.25 to 1.65%) when compared to base metal alloys.The shrinkage occurs in three stages.1)Thermal contraction of the liquid metal.2)Contraction of the metal while changing from liquid to solid state.3)Thermal contraction of solid metal as it reaches room temperature.Shrinkage affects the fit of the restoration. Therefore, it must be controlled and compensated for in the casting technique.
30 Biocompatibility Gold alloys are relatively biocompatible. Casting Investment Gypsum-bonded investments are used for gold alloys because of their lower fusion temperature.
31 HEAT TREATMENT OF GOLD ALLOYS Heat treatment of alloys is done in order to alter its mechanical properties. Gold alloys can be heat treated if it contains sufficient amount of copper. Only type I and type IV gold alloys can be heat treated.There are two types of heat treatment;1) Softening heat treatment (solution heat treatment) 2)Hardening heat treatment (age hardening).
32 Softening Heat Treatment: Softening heat treatment increases ductility, but reduces strength, proportions limit, and hardness. Indications :It is indicated for appliances that are to be ground, shaped or otherwise cold worked in or outside the mouth.Method :The casting is placed in an electric furnace for 10 minutes at 700°C, and then it is quenched in water. During this period, all intermediate phases are change to a disordered solid solution, and the rapid quenching prevents ordering from occurring during cooling. Each alloy has its optimum temperature. The manufacturer should specify the most favorable temperature and time.
33 Hardening Heat Treatment (or Ageing) Hardening heat treatment increases strength, proportional limit, and hardness, but decrease ductility. It is the copper present in gold alloys which helps in the age hardening process.IndicationsFor strengthening metallic dentures, saddles, bridges, and other similar structures before use in the mouth. It is not employed for smaller structures such as inlays.
34 MethodIt is done by "soaking" or ageing the casting at a specific temperature for a definite time, usually 15 to 30 minutes. It is then water quenched or cooled slowly. The ageing temperature depends on the alloy composition but is generally between 200C and 450°C. During this period, the intermediate phases are changed to an ordered solid solution (The proper time and temperature for age hardening an alloy is specified by its manufacturer). Ideally, before age hardening an alloy, it should first be subjected to a softening heat treatment in order to relieve all strain hardening (stresses which occurs during finishing). Starting the hardening treatment when the alloy is in a disordered solid solution allows better control of the ageing process.
35 low Gold AlloysAlso known as "economy golds". They are crown and bridge alloys having gold content below 60% (generally in the 42 to 55% range). However, gold must be the major element. The low gold alloys were developed because of the increase in gold prices. However, reducing gold content increased tarnish and corrosion. This problem was overcome by two discoveries.1)Palladium made the silver in gold alloy more tarnish resistant. 1% palladium was required for every 3% of silver.2)The silver-copper ratio had to be carefully balanced.
36 AdvantagesBecause of this research numerous low gold alloys were introduced into the market. Thus, these alloys were not only less expensive but also had good tarnish and corrosion resistance. Their properties are comparable to Type III and IV gold alloys.
37 SILVER-PAllADIUM AllOYS These alloys were introduced as a cheaper alternative to gold alloys. It is predominantly silver in composition. Palladium (at least 25%) is added to provide nobility and resistance to tarnish. They may or may not contain copper and gold. They are white in color.
38 Ag-Pd (non-copper)Ag - 70 to 72%Pd - 25%(Properties are like Type III gold alloys)Ag-Pd-Cu(Ag - 60%) (Pd - 25%) ( Cu - 15% )Properties are like Type IV gold alloys
39 The properties of the silver-palladium alloys are similar to the type III and IV gold alloys. However, they have lower ductility and corrosion resistance. They also have a significantly lower density than gold alloy. This may affect its castability. A major difference between type III and IV Ag-Pd alloys is that, the latter can be significantly age hardened, because of its gold and copper content.
40 NICKEL·CHROME AND COBALT·CHROMIUM ALLOYS These are known as base metal alloys and are extensively used in many of the developing countries. In India, because of their relatively low cost many of the laboratories use these alloys along with resin facings. These metals are very strong and hard. Because of this they are generally difficult to work with (cutting, grinding, polishing, etc).
41 TITANIUM AND TITANIUM ALLOYS Though these metals can be used for all-metal and metal ceramic restorations, as well as partial dentures.
42 ALUMINUM BRONZE ALLOYBronze is an alloy known to man since ancient times. Traditional bronze is copper alloyed with tin. The ADA approved bronze does not contain tin. The composition is as follows:Copper (81 to 88%) , Aluminum (8 to 10%)Nickel ( 2 to 4%) , Iron ( 1 to 4%).Being relatively new, the information on these alloys is relatively scanty.
43 METAL CERAMIC ALLOYSMetal ceramic alloys are those alloys that are compatible with porcelain and capable of bonding to it. A layer of porcelain is fused to the alloy to give it a natural tooth like appearance. Porcelain being a brittle material fractures easily, so these alloys are used to reinforce the porcelain.
44 Several types of alloys are used to cast sub-structures for porcelain fused to metal crowns and bridges. They may be noble metal alloys or base metal alloys. All have coefficient of thermal expansion (CTE) values which match that of porcelain. Note CTE has a reciprocal relationship with melting point, i.e. the higher the melting point of a metal, lower is its CTE.
45 SynonymsPorcelain-fused-to-metal (PFM), Ceramometal alloys, porcelain-bonded-to-metal (PBM). The preferred term however, is metal ceramic or PFM.
46 EVOLUTION OF METAL-CERAMIC ALLOYS The metal-ceramic alloys evolved from resin-veneered crown and bridge alloys. Resin facing faced the problem of gradual wear and had to be replaced over time. Besides resin could not be used on the occlusal surface. To retain a resin veneered restoration undercuts had to be provided. The early metal-ceramic alloys were high gold alloys (88% gold). They were not strong enough for use in bridges. In those early days before porcelain-metal bonding was clearly understood, porcelain had to be retained by mechanical means with the help of undercuts. Later, it was discovered that adding 1% of base metals like iron, tin, indium, etc. induced chemical bonding by the formation of an oxide layer. This significantly improved the bond strength between the porcelain and the metal
47 REQUIREMENTS OF ALLOYS FOR PORCELAIN BONDING In addition to the general requirements of alloys mentioned earlier, metal ceramic alloys have some special requirements in order to be compatible with porcelain veneering.1)It's melting temperature should be higher than the porcelain firing temperature.2)It should be able to resist creep or sag at these temperatures. 3)Its CTE should be compatible with that of porcelain. 4)They should be able to bond with porcelain.5) It should have a high stiffness (modulus of elasticity). Any flexing of the metal framework may cause porcelain to fracture.6) It should not stain or discolor porcelain.
48 USES OF METAL-CERAMIC ALLOYS 1)As the name implies these alloys are intended for porcelain veneered restorations (crowns and bridges).2)They can also be used as an all metal restoration.
49 TYPES (CLASSIFICATION) OF METAL CERAMIC ALLOYS Alloys for metal ceramics restorations may be categorized as:1)High noble (commonly referred to as gold alloys)a) Gold-palladium-platinum alloysb) Gold-palladium-silver alloysc) Gold-palladium alloys
50 2)Noble (commonly referred to as palladium alloys) Palladium-silver alloysPalladium-gallium-silver alloysPalladium-gold alloysPalladium-gold-silver alloysPalladium-copper alloysPalladium-cobalt alloys3)Base metalNickel-chromium alloysNickel-chromium-beryllium alloysCobalt-chromium alloysPure titaniumTitanium-aluminum-vanadium
51 THE HIGH NOBLE (GOLD BASED) METAL-CERAMIC ALLOYS As mentioned earlier, the high noble alloys contain more than 40 wt.% gold and are therefore also referred to as gold alloys or gold based alloys
52 Common Features of High Noble (Gold Based) Alloys Cost these are the most expensive crown and bridge alloys. However, in spite of the cost these alloys are user friendly and are preferred in practices where the clientele can afford the cost.Color the color can range from white to gold depending on the gold content. The whitening alloys are palladium and platinum. The gold color when present can enhance the vitality of the porcelain thus improving the esthetics
53 Melting range Porcelain is fired at a temperature of900 to 960°C Melting range Porcelain is fired at a temperature of900 to 960°C. Thus obviously these alloys must have melting temperatures much higher than the temperatures at which porcelain is fired. Pure gold has a melting temperature of l063°C. The melting temperature is raised by the addition of platinum (l769°C) and palladium (1552°C). The melting temperatures of these metal ceramic gold alloys range from 1149 to 1304°C.Density ranges from 13.5 to 18.3 gm/cm- (depending on the gold content). Because of the high gold and noble metal content, these alloys have a high density. The density reduces as more palladium is added.
54 Castability the high density of these alloys make them easy to cast Castability the high density of these alloys make them easy to cast. If done well one can expect most of the fine features to be accurately duplicated.Yield strength ranges from 450 to 572 MPa. Hardness and workability ranges from 182 to 220 VHN. These alloys are relatively softer when compared to the base metal alloys and so are extremely easy to work with. They are easy to cut, grind and polish.Percent elongation ranges from 5 to 20%. This gives an indication of the ductility of the alloy. The higher the value the more ductile it is.
55 Porcelain bonding the presence of an oxide layer on the surface of metal ceramic alloys assists in chemical bonding of porcelain to the alloy. Pure noble metal alloys rarely form an oxide layer. To induce the formation of an oxide layer, 1% of base metals like tin, indium, iron, etc. are added to the alloy. This significantly improved the bond strength between the porcelain and the metal.Sag resistance (It is the ability of dental alloy to resist plastic deformation and creep or flow under its own weight during porcelain firing and soldering) during porcelain firing, the metal frame has to withstand temperatures of as high as 950°C. At these high temperatures there is a danger of the metal substructure sagging under its own weight, thereby deforming. The longer the span the greater is the danger of sagging. The ability of a metal to resist sag is known as sag resistance. Compared to base metal alloys, gold alloys are less sag resistant.Tarnish and corrosion Because of their high noble metal content, these alloys are extremely stable in the oral environment. Noble metals have low reactivity to oxygen and therefore do not tarnish easily.
56 Biocompatibility high noble alloys have had a good and safe track record. They are not known to cause any problems in the mouth.Reusability these alloys are stable and so scrap from these alloys can be recast at least two or three times. However, the more volatile base metals like zinc, indium, tin, etc. may be lost. To compensate for this, equal amounts of new alloys should be mixed. The scrap should be cleaned by sandblasting and ultrasonic cleaning before use. Alloys from different manufacturers should not be mixed as it may change its composition and properties.Soldering Gold based alloys are quite easy to solder.
57 TYPESThe following three will be briefly described. Gold-palladium-platinum alloysGold-palladium-silver alloysGold-palladium alloys
58 Gold-Palladium-Platinum Alloys CompositionGold ( 80 to 88 wt%)Palladium (5 to 11 wt%)Platinum (6 to 8 wt%)Silver (0 to 4.9 wt%)Base metals ( balance around 1%)
59 Gold-Palladium-Silver Alloys CompositionGold (39 to 77 wt%)Palladium (10 to 44 wt%)Silver (9 to 22 wt%)Base metal (balance around 1%)The silver has a tendency to discolor some porcelains.
60 Gold-Palladium Alloys CompositionGold ( 44 to 55 wt%)Palladium (35 to 45 wt%0Base metals ( balance around 1%)The absence of silver eliminates the discoloration problem.
61 THE NOBLE (PALLADIUM BASED) METAL-CERAMIC ALLOYS By definition these alloys must contain at least 25% of noble metal alloy. Currently, the noble metal-ceramic alloys are mostly palladium based. The high cost of gold prompted the development of the cheaper base metal alloys. Unfortunately many soon became disillusioned because of the difficulty to work with these alloys (poor castability and high hardness). The palladium based alloys were developed during this period. Their properties were between that of the high noble alloys and the base metal alloys. They also had good scrap value.
62 Common Features of Palladium Based (Noble) Alloys Cost their cost range between that of the gold alloys and the base metal alloys.Color they are white in color.Density they are less denser than the gold alloys. The density ranges from 10.5 to 11.5 gm/cm",Castability these alloys have a lower density than the gold alloys and so do not cast as well. However, they are better than the base metal-ceramic alloys in this regard.
63 Workability like the gold alloys these alloys are extremely easy to work with. They are easy to cut, grind and polish.Melting range a typical melting range is 1155 to 1304°C. The melting range of these alloys like the gold ceramic alloys are high. This is desirable to ensure that these alloys don't melt during porcelain firing.Yield strength ranges from 462 to 685 MPa. These compare favorably with the high noble ceramic alloys which in turn compare favorably to the type IV alloys.Hardness ranges from 189 to 270 VHN. They tend to be slightly harder than the high noble metal ceramic alloys.
64 Percent elongation Ranges from 10 to 34% Percent elongation Ranges from 10 to 34%. This gives an indication of the ductility of the alloy. The higher the value the more ductile it is.Porcelain bonding Like the gold alloys, base metals like tin, indium, etc are added to assist porcelain bonding.Tarnish and corrosion Because of their high noble metal content, these alloys are extremely stable in the oral environment.Biological considerations These alloys are very safe and biocompatible.
65 TYPESThe following are the palladium based alloys Palladium-silver alloysPalladium-copper alloysPalladium-cobalt alloysPalladium-gallium-silver alloysPalladium-gold alloysPalladium-gold-silver alloys
66 Palladium-silver Alloys These alloys were introduced in the 1970's as an alternative to gold and base metal alloys. Their popularity has declined a little because of the greening problem.CompositionPalladium to 60 wt%Silver to 40 wt%Base metals balance( 1 to 8%)
67 Esthetics (Greening) The high silver content causes the most severe greening (greenish-yellow discoloration) problem among all the metal ceramic alloys. This must be kept in mind when using it for anterior teeth. Some manufacturers have provided special agents to minimize this effect (gold metal conditioners and coating agents). Another alternative is to use special non-greening porcelain
68 Palladium-Copper Alloys These are relatively new alloys. Little information is available regarding their properties.CompositionPalladium (74 to 80 wt%)Copper (5 to 10 wt%)Gallium (4 to 9 wt%)Gold (1 to 2 wt%)Base metal (around 1 wt%)
69 Esthetics Copper does cause a slight discoloration of the porcelain, but is not a major problem. During the oxidation firing the metal acquires a dark brown almostblack oxide layer. Care should be taken to mask this completely with opaquer. Also of concern is the dark line which develops at the margins.Castability These alloys are more technique sensitive. Slight errors can lead to faulty castings.
70 Palladium-Cobalt Alloys CompositionPalladium to 88 wt%Cobalt to 10 wt%Gallium up to 9wt%Base metals around 1 wt%Esthetics Cobalt can cause some insignificant discoloration. However, more care should be given for masking the dark oxide layer with opaque.Sag resistance They are the most sag resistant of all the noble alloys.
71 Palladium-Gallium Alloys There are two groups-the palladium-gallium-silver and the palladium-gallium silver-gold.CompositionPalladium 75 wt%Gallium 6 wt%Silver to 8 wt%Gold wt%Base metal around 1 wt%Esthetics The oxide layer though dark is still somewhat lighter than the palladium copper and palladium cobalt alloys. The silver content does not cause any greening.
72 BASE METAL ALLOYS FOR METAL CERAMIC RESTORATIONS Alloys which contain little or no noble metals are known as base metal alloys. As mentioned earlier, these alloys were introduced as a cheaper alternative to the very expensive noble metal ceramic alloys. In countries like the USA, western Europe and some middle eastern states, there is a preference for noble and high noble ceramic alloys. In contrast, developing countries have shown a preference for base metal-ceramic alloys. This is because the economic concerns far outweigh the advantages of the more user-friendly high noble alloys.
73 The first base metal alloys were the cobalt-chromium alloys primarily used for removable partial denture alloys. The nickel-chrome alloys were introduced later. The latest in the series are titanium and its alloys. Just like the gold alloys, the base metal alloys can be used for many purposes. However, one must differentiate between the ones used for all metal and the metal ceramic restorations. Obviously the metal-ceramic alloys would be formulated with special properties since they are to be used with ceramics.The following base metal alloys are used for metal-ceramics.Nickel-chromium (nickel based) alloysCobalt-chromium (cobalt based) alloyPure titaniumTitanium-aluminum-vanadium alloys
74 NICKEL-CHROMIUM ALLOYS Although cobalt chromium alloys are used for metal ceramic crowns and bridges, many laboratories prefer to use nickel-chromium alloys. For this reason the discussion will focus mostly on these alloys. Cobalt-chromium will be discussed later under alloys for removable dentures.
75 Composition Basic elements: Nickel 61 to 81 wt% Chrome 11 to 27 wt% Molybdenum 2 to 9 wt%
76 Some alloys occasionally contain one or more minor elements The minor additions includeNickel to 81 wt%Beryllium to 2.0 wt%Aluminum 0.2 to 4.2 wt%Iron to 0.5 wt%Silicon to 2.8 wt%Copper to 1.6 wt%Manganese 0.1 to 3.0 wt%Cobalt to 0.5 wt%Tin wt%The functions of each ingredient is described in the section on removable partial denture alloys
77 General Features and of Nickel Based Alloys Cost they are the cheapest of the casting alloys. Color They are white in color.Melting range a typical melting range is 1155 to 1304°C. The melting range of these alloys like the gold ceramic alloys are high.Density ranges from 7.8 to 8.4 gm/cm-'. They have just half the density of the gold alloys making them much lighter. One can get more castings per gram compared to the gold alloys.
78 Castability they are extremely technique sensitive Castability they are extremely technique sensitive. One reason may be their lower density compared to the gold alloys.Hardness and workability ranges from 175 to 360 VHN. They tend to be much harder than the high noble metal ceramic alloys. Unlike the gold alloys these alloys are extremely difficult to work with. Their high hardness makes them very difficult to cut (sprue cutting), grind and polish. In the mouth more chair time may be needed to adjust the occlusion. Cutting and removing a defective crown can be quite demanding. The high hardness results in rapid wear of carbide and diamond burs. Yield strength ranges from 310 to 828 MPa. These alloys are stronger than the gold and palladium based alloys.
79 Modulus of elasticity ranges from 150 to 210 MPa This property denotes the stiffness of the alloy. Base metal alloys are twice as stiff as the gold ceramic alloys. Practically, this means that we can make thinner, lighter castings or use it in long span bridges where other metals are likely to fail because of flexing. Gold alloys require a minimum thickness of at least 0.3 to 0.5 mm, whereas base metal alloys copings can be reduced to 0.3 mm (some even claim 0.1 mm).Percent elongation ranges from 10 to 28%. This gives an indication of the ductility of the alloy. Though they may appear to be ductile these alloys however, are not easily burnishable. This may be related to additional factors like the high hardness and yield strength
80 Porcelain bonding These alloys form an adequate oxide layer which is essential for successful porcelain bonding. However, occasionally the porcelain may delaminate from the underlying metal. This has been blamed on a poorly adherent oxide layer which occurs under certain circumstances which have not been fully understood.Sag resistance These materials are far more stable at porcelain firing temperatures than the gold based alloys. They have a higher sag resistance.EstheticsA dark oxide layer may be seen at the porcelain metal junction.Tarnish and corrosion resistanceThese alloys are highly resistant to tarnish and corrosion. This is due to the property known as passivation. Passivation is the property by which a resistant oxide layer forms on the surface of chrome containing alloys. This oxide layer protects the alloy from further oxidation and corrosion. These alloys can maintain their polish for years. Other self passivating alloys are titanium and aluminum.
81 Soldering Soldering is necessary to join bridge parts Soldering Soldering is necessary to join bridge parts. Long span bridges are often cast in two parts to improve the fit and accuracy. The parts are assembled correctly in the mouth and an index made. The parts are then reassembled in the laboratory and joined together using solder. Base metal alloys are much more difficult to solder than gold alloys. Casting shrinkage These alloys have a higher casting shrinkage than the gold alloys. Greater mould expansion is needed to compensate for this. Inadequate compensation for casting shrinkage can lead to a poorly fitting casting.Etching Etching is necessary for resin bonded restorations (e.g. Maryland bridges) to improve the retention of the cement to the restoration. Etching of base metal alloys is done in a electrolytic etching bath.Biological considerations Nickel may produce allergic reactions in some individuals. It is also a potential carcinogen. Beryllium which is present in many base metal alloys is a potentially toxic substance. Inhalation of beryllium containing dust or fumes is the main route of exposure. It causes a condition known as 'berylliosis'. It is characterized by flulike symptoms and granulomas of the lungs.Caution Adequate precautions must be taken while working with base metal alloys. Fumes from melting and dust from grinding alloys should be avoided (wear mask). The work area should be well-ventilated. Good exhaust systems should be installed to remove the fumes during melting.
82 TITANIUM AND ITS ALLOYS Recently titanium and its alloys have become available for use in metal-ceramics. It is also used for removable partial denture alloy frames and of course commercial implants, It has been adapted in dentistry because of its excellent biocompatibility, light weight, good strength and ability to passivate.
83 Uses in Dentistry 1)Metal ceramic restorations 2)Dental implants 3)Partial denture frames4)Complete denture bases5) Bar connectors(In dentistry it is especially useful as an alternative alloy to those who are allergic to nickel
84 Properties of Commercially Pure Titanium Color it is a white color metal Density It is a light weight metal (density 4.1 gm/cm-) when compared to nickel chrome (8 gms/cm-) and gold alloys (15 gm/cm"). Modulus of elasticity its MOE is 110 MPa which makes it only half as rigid as base metal alloys. However this appears to be sufficient for most dental uses.
85 Melting point its melting point is quite high (1668°C) Melting point its melting point is quite high (1668°C). Special equipment is needed for casting titanium.Coefficient of thermal expansion this is an important property when it is used as a metal ceramic alloy. When used as a metal ceramic alloy the CTE is far too low to be compatible with porcelain. For this reason special low fusing porcelains have been developed to get around this problem.Biocompatibility It is nontoxic and has excellent biocompatibility with both hard and soft tissues.Tarnish and corrosion Titanium has the ability to self-passivate. It forms a thin protective oxide layer which protects the metal from further oxidation.
86 Casting InvestmentsDue to the high melting temperature of these alloys, only phosphate-bonded or silica-bonded investments are used. However, in case of gold based metal-ceramic alloys, carbon containing phosphate bonded investments are preferred.
87 REMOVABLE DENTURE ALLOYS Larger structures like complete denture bases and partial denture frames are also made from dental alloys. Obviously these would need large amounts of alloy, which can make them quite heavy and expensive (if gold were to be used). Thus it became necessary to develop lighter and more economical alloys. Most of the large castings today are made from base metal alloys, occasionally type IV gold alloys are used.
88 Additional Requirements for Partial Denture Alloys Besides all the earlier mentioned general requirements of casting alloys, RPD alloys have a few special requirements.1)They should be light in weight. Being much larger structures the lighter weight aids in retention in the mouth.2)They should have high stiffness. This aids in making the casting more thinner. This is important especially in the palate region where having a thin palatal portion makes it more comfortable to the patient. The high stiffness prevents the frame from bending under occlusal forces.
89 3)They should have good fatigue resistance 3)They should have good fatigue resistance. This property is important for clasps. Clasps have to flex when inserted or removed from the mouth. If they do not have good fatigue resistance they may break after repeated insertion and removal. 4)They should be economical. Large structures would require more metal and therefore the cost of the alloy should be low.5)They should not react to commercial denture cleansers.
90 Types The alloys for removable denture use are Cobalt chromium Nickel chromiumAluminum and its alloysType IV noble alloys
91 COBALT CHROMIUM ALLOYS Cobalt-chromium alloys have been available since the 1920's. They possess high strength. Their excellent corrosion resistance especially at high temperatures makes them useful for a number of applications. These alloys are also known as 'stellite' because of their shiny, star-like appearance. They have bright lustrous, hard, strong, and non-tarnishing qualities.
92 APPLICATIONS APPLICATIONS 1)Denture base 2)Cast removable partial denture framework3)Crowns and bridges4)Bar connectors
93 Composition Cobalt 35 to 65% Chromium 23 to 30 % Nickel 0 to 20 % Molybdenum 0 to 7 %Iron to 5 %Carbon up to 0.4 %Tungsten, manganese, silicon and platinum in traces. According to ADA Sp. No. 14 a minimum of 85% by weight of chromium, cobalt, and nickel is required.
94 FUNCTIONS OF ALLOYING ELEMENTS Cobalt Imparts hardness, strength and rigidity to the alloy. It has a high melting point.Chromium Its passivating effect ensures corrosion resistance. The chromium content is directly proportional to tarnish and corrosion resistance. It reduces the melting point. Along with other elements, it also acts in solid solution hardening. 30% chromium is considered the upper limit for attaining maximum mechanical properties.
95 Nickel Cobalt and nickel are interchangeable Nickel Cobalt and nickel are interchangeable. It decreases strength, hardness, MOE and fusion temperature. It increases ductility.Molybdenum or Tungsten They are effective hardeners. Molybdenum is preferred as it reduces ductility to a lesser extent than tungsten. Molybdenum refines grain structure.Iron, Copper, Beryllium They are hardeners. In addition, beryllium reduces fusion temperature and refines grain structure.Manganese and Silicon Primarily oxide scavengers to prevent oxidation of other elements during melting. They are also hardeners.
96 Boron Deoxidizer and hardener, but reduces ductility. Carbon Carbon content is most critical. Small amounts may have a pronounced effect on strength, hardness and ductility. Carbon forms carbides with the metallic constituents which is an important factor in strengthening the alloy. However, excess carbon increases brittleness. Thus, control of carbon content in the alloy is important.
97 PROPERTIESThe cobalt-chromium alloys have replaced Type IV gold alloys especially for making RPDs because of their lower cost and good mechanical properties.Density The density is half that of gold alloys, so they are lighter in weight (8 to 9 gm\ cm").
98 Fusion Temperature Thus casting temperature of this alloy is considerably higher than that of gold alloys (l250°C to 1480°C). ADA Sp. No. 14 divides it into two types, based on fusion temperature, which is defined as the liquidus temperature. Type-I (high fusing)-liquidus temperature greater than 1300°C. Type-ll (low fusing)-liquidus temperature not greater than 1300°C.Yield Strength It is higher than that of gold alloys (710 MPa).
99 Elongation Their ductility is lower than that of gold alloys Elongation Their ductility is lower than that of gold alloys. It depends on composition, rate of cooling, and the fusion and mould temperature employed. The elongation value is 1 to 12%.Caution care must be taken while adjusting the clasp arms of the partial denture. They may break if bent too many times.Modulus of Elasticity They are twice as stiff as gold alloys (225 x 10" MPa). Thus, casting can be made thinner, thereby, decreasing the weight of the RPD.
100 Hardness These alloys are 50% harder than gold alloys (432 VHN) Hardness These alloys are 50% harder than gold alloys (432 VHN). Thus, cutting, grinding and finishing is difficult. It wears off the cutting instrument. Special hard, high speed finishing tools are needed.Tarnish and Corrosion Resistance (Passivation) Formation of a layer of chromium oxide on the surface of these alloys prevents tarnish and corrosion in the oral cavity. This is called 'passivating effect'. Caution Hypochlorite and other chlorine containing compounds that are present in some denture cleaning solutions will cause corrosion in base metal alloys. Even the oxygenating denture cleansers will stain such alloys. Therefore, these solutions should not be used to clean chromium based alloys.Casting Shrinkage The casting shrinkage is much greater (2.3%) than that of gold alloys. The high shrinkage is due to their high fusion temperature.Porosity as in gold alloys, porosity is due to shrinkage of the alloy and release of dissolved gases. Porosity is affected by the composition of the alloys and its manipulation.
101 Technical considerations for casting alloys Based on the melting temperatures of the alloys we can divide the alloys into high fusing and low fusing alloys.
102 Low fusing alloysThe gold alloys used for all-metal restorations may be considered as low fusing. Obviously the technical requirements of these alloys would be different from the high fusing alloys.Investment materials Gypsum bonded investments are usually sufficient for the low fusing gold alloys.Melting the regular gas-air torch is usually sufficient to melt these alloys
103 High fusing alloysThe high fusing alloys include noble metal ceramic alloys ( gold and palladium alloys)As well as the base metal alloys ( all metal, metal-ceramic alloys and partial denture alloys.Investment materials for noble metal alloysThe high melting temperatures prevent the use of gypsum bonded investments. phosphate bonded or silica bonded investments are used for these alloys.
104 Investment material for base metal alloys phosphate bonded or silica bonded investments are also used for these alloys. However, there is one difference. Theses alloys are very sensitive to a change in their carbon content. Therefore, carbon containing investments should be avoided when casting base metal alloys.Burnout a slow burnout is done at a temperature of 732 to 982C. It is done two hours after investing.
105 Melting the high fusion temperature also prevents the use of gas-air torches for melting these alloys. Oxygen-acetylene torches are usually employed. Electrical sources of melting such as carbon arcs, argon arcs, high frequency induction, or silicon-carbide resistance furnaces, may also be used.
106 Technique for small castings The wax pattern is usually constructed on a die stone model. The wax pattern is removed and then invested .
107 Technique for large castings The procedure for large casting like RPD frames is slightly more complex. Unlike the crown or bridge pattern. The RPD pattern is difficult to remove from the model without distortion and damage. Therefore a modification in the technique is required. A duplicate of the model is made using investment material (this called refractory cast). The wax pattern is constructed on the refractory cast. The pattern is not separated from the refractory cast, instead the refractory cast is invested along with the pattern.
108 Advantages of base metal alloys 1) Lighter in weight.2) Better mechanical properties3) As corrosion resistant as gold alloys (due to passivating effect).4) Less expensive than gold alloys.
109 Disadvantages 1) More technique sensitive. 2) Complexity in production of dental appliance.3) High fusing temperatures.4) Extremely hard, so required special equipment for finishing.5) The high hardness can cause excessive wear of restorations and natural teeth contacting the restorations.